An In vitro Comparative Evaluation of Flexural Strength of Monolithic Zirconia after Surface Alteration Utilising Two Different Techniques
Ketaki Janardhan Chougule1, Arti Prabodh Wadkar2
ABSTRACT Introduction: Chairside surface alteration like grinding is often done by clinicians for adjustment of zirconia restorations. To restore the surface of the prostheses, either polishing or glazing is done. However, there is a controversy which of the surface restoration technique helps regain strength of the restoration.
and polished (n=10) and third was ground and reglazed (n=10). Flexural strength testing was performed with a three-point bend test on a universal testing machine. The collected data was statistically analysed for normal distribution using D'Agostino and Pearson omnibus normality test, one-way ANOVA and Tukeys multiple comparison test (p 0.05 non significant)
15 mm . The ultimate load that caused specimen fracture was recorded [Table/Fig-6a-c]. Mean fracture strengths were calculated using the following equation as recommended by the ISO 6872 standard, 1995 . M= 3WI/2bd2 Where, M=Flexural strength (Mpa), W=fracture load (N), I =test span (center to center) distance between support points (mm), b=breadth of specimen (mm), d=thickness of specimen. Details of the test materials are given in [Table/Fig-7].
Quantitative data was presented in the form of mean, standard deviation and median [Table/Fig-8a]. Tests used were one-way ANOVA as per the results of D’Agostino and Pearson omnibus normality test [Table/Fig-8b] and [Table/Fig-9] Tukey’s multiple comparison test [Table/Fig-10].
blunting the flaw tips thereby increasing the strength. Second could be due to the fact that overglaze layer has a lower thermal expansion coefficient than the leucite-rich interior. This places the outer surface in compression when cooled. Applying this knowledge to zirconia based ceramics, the current study was performed, in which the strength of the reglazed group increased as compared to the control group. Iseri U et al., concluded that all grinding procedures decreased the flexural strength . In their study, temperature obtained by micromotor grinding was significantly higher than high-speed handpiece grinding because low speed produce more heat. Lesser the heat more is the flexural strength due to retention of the monoclinic phase. Hence, grinding zirconia with low speed handpiece decreased flexural strength whereas high-speed caused the least reduction in strength. In the current in vitro study, a water spray was used as a coolant reducing the temperature thus decreasing the effect of temperature variations on the strength. Iseri U et al., concluded that although grinding influenced the flexural strength of zirconia, it was not statistically significant . Nakamura Y et al., also performed a study in which they concluded that the mean flexural strength of the glazed group was the highest, while that of the polished groups was low . The crack inhibition phenomenon was responsible for this result. However, Yener ES et al., in their study investigated the effect of glazing and concluded that glazing decreased the flexural strength significantly . Unglazed specimens had more flexural strength than that of glazed. They gave two possible explanations for their conclusion. One was the manufacturing process causing compressive stresses on the surface which was relieved by heat treatment and veneering. Other would be due to monoclinic to tetragonal (m to t) phase transformation or change in particle size during heat treatment or veneering. Aboushelib M et al., observed variations in their study in which they concluded that strength increased statistically in polishing as the fine surface flaws were eliminated . Glaze porcelain caused less regain in strength because of poor wetting ability and high viscosity failing to seal the deep flaws. The research hypothesis for this in vitro study was that there was no difference in the flexural strength after surface alterations. However, this hypothesis was rejected following the study, since there were statistically significant differences after surface alterations.
[Table/Fig-8a] showing the mean flexural strengths of the three groups. The strength of the reglazed group was found to be higher as compared to other groups.
The effect of temperature variations, sand blasting, heat treatment, variable speeds and ageing were not taken into consideration. This study was performed only on one brand but further studies including more number of brands along with long term clinical trials are required to substantiate the results obtained in this study.
Studies have shown that grinding can introduce compressive stresses which inhibit crack propagation increasing the flexural strength of zirconia . Studies on this aspect have proven that restoration of surface damage improved the flexural strength of zirconia specimens . Grinding promotes tetragonal to monoclinic (t to m) form transformation. Monoclinic being a more stable form of zirconia, causes an increase in the strength of zirconia. However, few studies have revealed that fine polishing lowers the mean flexural strength by removing the layer of compressive stresses [7,18]. This explained why greater strength was not found for the polished specimen. The results of this study are similar to previous studies in which the influence of grinding and polishing on the flexural strength of zirconia was investigated .
Flexural strength was found to be increased after reglazing and polishing treatment as compared to the control. The effect of glazing on the flexural strength of zirconia was found to be statistically significant and that of polishing was non-significant. Clinicians can provide improved, high strength restorations to the patients without fearing the reduction in strength after performing any alterations. Accurate impression techniques, precise fabrication and lab finishing procedures would reduce the effort of chairside alterations thus decreasing the complications associated with fractured restorations. High translucency monolithic zirconia is also developed recently which could be used in anterior restorations without fearing the opacity of conventional zirconia.
Chang I et al., stated that overglazed group had significantly higher flexural strength than self-glazed and polished group, whereas there was not much difference between the glazed and polished group . The high flexural strength in the overglazed group may have been due to two possible explanations. First one was due to the overglazed layer filling the surface flaws and subsequently
 Anusavice KJ. Phillips' Science Of Dental Materials. 12th ed. USA: Elsevier; 2013.  Fernando Z, Russo S. From porcelain-fused-to-metal to Zirconia: Clinical and experimental considerations. Dent Mater. 2011;27:83-96.  Raigrodski AJ. Contemporary all-ceramic fixed partial dentures: A review. Dent Clin N Am. 2004;48:531-44. Journal of Clinical and Diagnostic Research. 2017 Aug, Vol-11(8): ZC20-ZC23
Ketaki Janardhan Chougule and Arti Prabodh Wadkar, Comparative Evaluation of Flexural Strength of Monolithic Zirconia after Surface Alteration
 Piwowarczyk A, Ottl P, Lauer H, Kuretzky T. A clinical report and overview of scientific studies and clinical procedures conducted on the 3M ESPE Lava All ceramic system. J Prosthodont. 2005;14:39-45.  Mafda A, Al-Sanabani F, Al-Qudami N, Al-Sanabani J, Amran A. Use of zirconia in dentistry: an overview. The Open Biomaterials Journal. 2014;5:1-9.  Denry I, Kelly JR. State of the art of zirconiafor dental applications. Dent Mater. 2008;24:299-307.  Kelly RJ, Denry I. Stabilized zirconia as a structural ceramic: An overview. Dent Mater. 2008;24:289-98.  Komine F, Strub JR, Matsumura H. Bonding between layering materials and zirconia frameworks. Jpn Dent Sci Rev. 2012;48:153-61.  Beuer F, Stimmelmayr M, Gueth JF, Edelhoff D. In vitro performance of fullcontour zirconia single crowns. Dent Mater. 2012; 28:449-56.  Zhang Y, Lee JJ, Shrikant R, Lawn BR. Edge chipping and flexural resistance of monolithic ceramics. Dent Mater. 2013;29:1201-08.  Jeffries S. Abrasive finishing and polishing in restorative dentistry: A state-of-theart review. Dent Clin N Am. 2007;51:379-97.  Miyazaki T, Hotta Y, Kunii J, Kuriyama S, Tamaki Y. A review of dental CAD/CAM: Current status and future perspectives from 20 years of experience. Dent Mater. 2009;28(1):44-56.  American National Standard /American Dental Association Specification number 69 for Dental Ceramic. In; 1991.
 Iseri U, Ozkurt Z, Kazazoglu E, Kucukoglu D. Influence of grinding procedures on the flexural strength of zirconia ceramics. Braz Dent J. 2010;21(6):528-32.  Aboushelib M, Wang H. Effect of surface treatment on flexural strength of zirconia bars. J Prosthet Dent. 2010;104(2):98-104.  Wang H, Aboushelib M, Feilzer A . Strength influencing variables on CAD/CAM zirconia frameworks. Dent Mater. 2008;24:633-38.  International Organization for Standardization ISO 6872(E): Dental ceramics. In; 1995.  Guzzato M, Albakry M, Quach L, Swain M. Influence of surface and heat treatments on the flexural strength of a glass infiltrated alumina/ zirconiareinforced dental ceramic. Dent Mater. 2005;21:454-63.  Chang I, Lee S, Yang J, Han J, Lee J . The effect of surface finishes on flexural strength, fracture toughness on feldspathic dental porcelain. J Korean Acad Prosthodont. 2005;43:293-303.  Iseri U, Ozkurt Z, Yalniz A, Kazazoglu E. Comparison of different grinding procedures on the flexural strength of zirconia. J Prosthet Dent. 2012;107:30915.  Nakamura Y, Hojo S, Sato H. The effect of surface roughness on Weibull distribution of porcelain strength. Dent Mater. 2010;29(1):30-34.  Yener ES, Ozcan M, Kazazoglu E. The effect of glazing on the biaxial flexural strength of different zirconia core materials. Acta Odontol Latinoam. 2011;24:13340.
PARTICULARS OF CONTRIBUTORS: 1. Ex-Postgraduate Student, Department of Prosthodontics, Nair Hospital Dental College, Mumbai, Maharashtra, India. 2. Dean and Professor and Head, Department of Prosthodontics, Nair Hospital Dental College, Mumbai, Maharashtra, India. NAME, ADDRESS, E-MAIL ID OF THE CORRESPONDING AUTHOR: Dr. Ketaki Janardhan Chougule, 390 Elan Village Ln. # 320, San Jose, CA 95134, USA. E-mail : Ketsch[email protected]
Financial OR OTHER COMPETING INTERESTS: None.
Journal of Clinical and Diagnostic Research. 2017 Aug, Vol-11(8): ZC20-ZC23
Date of Submission: Nov 02, 2016 Date of Peer Review: Dec 22, 2016 Date of Acceptance: Apr 07, 2017 Date of Publishing: Aug 01, 2017